Domain Reversal and Wall Structure of 180 Ferroelectric ... reversal · PDF file Domain...
Embed Size (px)
Transcript of Domain Reversal and Wall Structure of 180 Ferroelectric ... reversal · PDF file Domain...
Domain Reversal and Wall Structure of 180°°°° Ferroelectric Domains in LiTaO3 Crystals
Venkatraman Gopalan*, K. Kitamura†, Y. Furukawa†
*Materials Research Laboratory and Dept. of Materials Science and Engineering, Pennsylvania State University, University Park, PA 16802
†National Institute for Research in Inorganic Materials, 1-1 Namiki, Tsukuba, 305-0044 Japan
Abstract. We report a dramatic influence of lithium nonstoichiometry in LiTaO3 crystals on the 180° coercive fields, internal fields, domain wall strain, optical birefringence, and domain shape. Congruent composition of LiTaO3 ( [Li]/([Li]+[Ta])~0.485) show large coercive fields of ~21kV/mm for domain motion and built-in internal fields of ~4.5kV/mm, domain wall strains of εzz~(1-10)x10-6, optical birefringence in the z-plane, and triangular domains with domain walls parallel to the crystallographic x-axes. On the other hand, near-stoichiometric crystals of LiTaO3 ([Li]/([Li]+[Ta])~0.499) studied here show low coercive fields of ~1.7kV/mm, internal fields of
Figure 1 shows the hysteresis loops for domain reversal at room temperature for congruent and stoichiometric crystals of z-cut LiTaO3.
Figure 1. Hysteresis loops of congruent and stoichiometric LiTaO3 crystals at room temperature. The Eint , indicated by the arrow, depicts the internal field as measured by the offset in the hysteresis loop for the congruent crystals. The crystals are cycled starting from state I through state II and back to state I.
The congruent LiTaO3 had a lithium concentration of [Li]/([Li]+[Ta])~0.485, whereas, the near-stoichiometric composition used in this study had [Li]/([Li]+[Ta])~0.499. Starting from a single crystal, single domain wafer, the domains were reversed using liquid electrodes (saturated salt solution of KNO3 in water) . Starting from state I, the polarization was reversed to state II (forward poling) and then back to state I (reverse poling). The coercive field for forward poling (Ef) and reverse poling (Er), were respectively ~21 kV/mm and ~12 kV/mm for congruent crystal. The difference reflects a large built-in internal field in the form of the offset of the hysteresis loop along the field axis, given by Eint= (Ef-Er)/2 ~4.5k V/mm. In the stoichiometric crystals , the coercive fields were Ef~1.7 kV/mm and Er~1.5 kV/mm, resulting in an Eint ~0.1 kV/mm. Clearly, there is a strong correlation between the presence of internal field and the lithium deficiency in the crystals. This is also
accompanied by an increase in the coercive field values in congruent crystals by an order of magnitude.
Figure 2 shows the change in the coercive fields as a function of temperature for both congruent and stoichiometric LiTaO3 crystals. The coercive field in congruent crystals shows a sharp decrease by a factor of 4 from room temperature (22°C) to 250°C . This is accompanied by a broadening of the range of electric fields over which domain reversal takes place, and the disappearance of internal fields at 250°C. The dc conductivity of the crystal also increases exponentially as a function of temperature with activation energy of 0.66 ±0.14 eV. On the other hand, the stoichiometric crystals show little change in the coercive field over the entire range as shown.
FIGURE 2. The coercive field for domain reversal for congruent (CLT) and stoichiometric (SLT) LiTaO3 crystals. The symbol notation is as follows: Filled squares: Ef-start (CLT); Open squares: Ef-end (CLT); Filled circles: Er-start (CLT); Open circles: Er-end (CLT); Open rhombus: Ef (SLT); Star: Er (SLT); filled rhombus: dc conductivity (CLT). The solid line fit to dc-conductivity is an exponential fit with activation energy of 0.66±0.14 eV.
The current understanding of the defect chemistry in nonstoichiometric LiTaO3 crystals is consistent with a charge balance between tantalum antisites ([TaLi]4+) and four lithium vacancies (4[Vli]-) [9, 10]. Evidence from diffuse X-ray scattering, [11, 12] neutron scattering,  and Nuclear Magnetic Resonance (NMR) measurements [14, 15] point to the likelihood of these point defects forming dipolar clusters ordered along
the Lithium and tantalum chains in the pseudo-cubic directions of the crystal. Based on these studies, we present a qualitative model to visualize the changes in coercive and internal fields seen above in terms of point defect complexes. Figure 3 shows a schematic of the stable states for the possible defect dipole for an “up” and a “down” domain, the notation referring to the polarization direction, Ps.
+y +z +z +y
FIGURE 3. Schematic describing a plausible model for the stable states of a 4[VLi]- -[TaLi]4+ dipolar defect in an “up” domain (a) and in a “down” domain (b). In this model, upon domain reversal at room temperature from +Ps in (a), to -Ps in (b) , the tantalum antisite ion (TaLi) moves from its position in (a) to that in (b). However, the lithium vacancies (VLi) remain in their original positions in (a), resulting in a “frustrate state” of the defect dipole. To achieve the stable state of defect dipole in (b), thermal activation is required by heating over 150°C.
The position of the lithium vacancy with respect to tantalum antisite has been arbitrarily chosen here assuming that defect dipole formed by [Vli]-- [TaLi]4+ along the z- axis orients parallel to the matrix polarization (Ps). When the Ps is reversed using electric field at room temperature from Fig. 3 (a) to Fig. 3(b), the lithium atoms, and the tantalum atom at the antisite is forced through the close packed oxygen triangle to a position just below the oxygen plane. The field-induced motion of the tantalum antisite across the oxygen plane may be responsible for the increase in the coercive field in congruent crystals. However, it appears that the lithium vacancies surrounding the antisite do not move under the electric field at room temperature. In this state, the
defect dipole at room temperature is in a “frustrated state” after domain reversal at room temperature. After heating the crystal to 150°C and above, the lithium ions are known to become increasingly mobile resulting in increase in the ionic conductivity seen in Fig. 2. This results in a randomization of the lithium vacancies in the lattice, and the disappearance of the defect dipole and hence the internal fields at higher temperatures. On cooling the crystal back, the lithium ions reorder to form a defect dipole in the opposite direction as shown in Fig. 3(b), resulting in the re-establishment of large internal fields and increased coercive fields at room temperature .
Domain Wall Strain and Optical Contrast
We present experimental evidence that suggest that the “frustrated defect dipoles” arising from lithium deficiency as proposed above also give rise to large regions of strain and optical birefringence adjacent to domain walls in congruent LiTaO3 crystals. These effects disappear in upon heating and cooling of the congruent crystals as well as in stoichiometric crystals. Figure 4 shows the optical image of domains created in congruent LiTaO3 at room temperature using electric field. The image is taken looking down the z-axis of the crystal,
FIGURE 4. An optical image of the z-plane 180° domains in congruent LiTaO3 taken with sample between cross-polarizers aligned along the horizontal and vertical axes of the above image. The polarization directions, Ps is normal to the image plane, and crystallographic +y-axis in the matrix domain points upwards along the vertical axis of the above image. Domain walls are parallel to the crystallographic x-axes. The triangular domains are formed by domain walls aligned along the crystallographic x-axes which are perpendicular to the three c-glide planes. In this crystal state, the
dipolar defects in Fig. 3 would be in a “frustrated state” inside the triangular domains, and in stable state outside the triangles . The transition region across a domain wall shows optical contrast. Since the image is taken with the sample between cross polarizers, and the crystal is optically isotropic in the z-plane, the image is mostly dark. However, light appears to leak through regions adjacent to the domain walls, which are at an angle to the polarizer and the analyzer, suggesting that these regions exhibit optical birefringence. The contrast disappears for walls which are parallel or perpendicular to the cross polarizers (for example the horizontal wall of the triangles in Fig. 4), thus revealing that the optical birefringence is between the refractive indices parallel (nx) and perpendicular (ny) to the domain walls. This birefringence has been carefully measured by Yang and Mohideen [18, 19] using Near-field Scanning Optical Microscope (NSOM) as nx-ny~ (2-10)x10-5 over widths ranging from 0.5-3 µms. Since this birefringence has contributions from strains directly through the elasto-optic effect and indirectly through the combination of piezoelectric and electro-optic effects, one can deduce the strains εy-εx~ 1.4x10-4 and εyz ~2x10-4 in the region of optical birefringence. This also corresponds to an electric field Ey~±10 kV/mm locally in the birefringence region. Yang and Mohideen  have also measured a surface step at the wall, corresponding to an approximate strain εzz ~ 1x10-6 and an electric field Ez ~0.15 kV/mm. If this electric field is multiplied by the relative dielectric constant,(k~45) it would correspond to the equivalent external electric field of kEz~6.75 kV/mm whic